### Interdiffusion in non-ideal systems Robert Filipek

*AGH University of Science and Technology *
*Faculty of Materials Science and Ceramics *

*Department of Solid State Chemistry *
*al. Mickiewicza 30, 30-059 Krakow, Poland *

* Fax: +48 12 6172493 *
*E-mail: rof@agh.edu.pl *

### Abstract

Darken’s method of interdiffusion for multi-component systems is presented. A postulate that the total mass flow is a sum of the diffusion and the drift flows, is applied for the description of interdiffusion in the bounded open system. Nernst-Planck’s flux formula assuming a

chemical potential gradient as a driving force for the mass transport is used for computation of the diffusion flux in non-ideal multi-component systems. An idea of the generalized solution was applied for obtaining the solution to the problem. Numerical solution using finite element method (Galerkin’s approximation) is shown. Applications of the model describing

interdiffusion in the Cu-Fe-Ni non-ideal alloys including diffusion mixing in the closed systems and the evolution of an alloy composition due to selective oxidation (open system) are presented.

### Introduction

Modelling of interdiffusion in multi-component systems has broad applicability in the materials science and engineering. Most of the modern materials used in advanced

technologies are multi-component and multi-phase. The diffusion processes in multi- component alloys influence the thermal stability and lifetime of electrical contacts, brazed joints and the durability of high temperature coatings. The understanding of the mechanisms of the mass transport in such complex materials is critical for achieving theirs optimal mechanical and physico-chemical properties for special applications. A theoretical approach for the description of interdiffusion in multi-component and non-ideal alloys is presented below.

For the phenomenological description of interdiffusion problem let us consider

isothermal and isobaric multi-component single-phase region in which diffusion occurs in one direction only (Figure 1). The two alloys of different composition and/or components are joined together to form a diffusion couple (Figure 1a). From now on the components start to diffuse from the region where theirs concentration is higher to the lower one (Figure. 1b).

When any compound interacts with a field, resulting in a gradient of chemical potential, the
different elements respond in different ways. In case of multi-component solutions the force
being a result of chemical potential gradient causes the atoms of the particular component to
move with a velocity υ* _{i}*, which may differ from the velocity of the atoms of the other
elements. Because the system is common for the components all the fluxes are coupled and
their local changes may affect the common system drift velocity υ . This phenomenon is
called interdiffusion [1]. Because of interdiffusion the concentration profiles of all
components are affected. At the end of the process in the finite system a homogeneous
solution is formed (Figure 1c).

The phenomenological description of diffusion process proposed by Onsager [2] and developed by Kirkaldy [3,4], Dayananda [5,6], van Loo [7,8], Morral [9,10] and others [11,12] dominates interdiffusion studies. Investigations of multi-component diffusion based on the Onsager concept are usually restricted to the determination of interdiffusion

coefficients and fluxes in ternary systems [4]. One can find only few applications for quaternary systems [6,13,14]. The use of Onsager phenomenology for more than four- component systems is unattainable due to the serious theoretical and experimental obstacles [13,15]. The Onsager phenomenological scheme is useful in describing the diffusion in the closed system. In the open system the translation velocity usually does not vanish [16] and consequently interdiffusion in the multi-component open system can not be described by a simple extension of the methods currently used.

A different method to describe interdiffusion was proposed by Darken [1]. In his model he assumed that the total mass flux is a sum of the diffusion flux and the drift flux. The drift velocity is a physical (real) velocity of an "ideal" marker placed in the diffusion zone.

This velocity gives rise to so called Kirkendall effect [17]. In this paper Darken’s method for multi-component non-ideal open systems is presented. The equations of mass conservation, the postulate of constant molar volume of the system and the appropriate initial and boundary conditions allow computing the concentration profiles of the components and the drift

velocity in the interdiffusion zone. The main advantages of this method are the generalized initial and boundary conditions, which allow the quantitative analysis of the interdiffusion process for the arbitrary initial concentration profiles of the components in the open as well as in the closed systems.

Formulation of the model describing interdiffusion in the ideal closed [18,19] and ideal open systems [20] as well as for non-ideal closed systems [21] have been already published. In this paper the mathematical model of interdiffusion in multi-component non- ideal open system is formulated and method of its solution is presented. A possible answer to such problem is based on the more general diffusion flux formula. It is postulated that the diffusion flux is more adequately described by Nernst-Planck equation [22].

### Formulation of the Model

In this section formulation of the model, i.e., the initial boundary-value problem for the interdiffusion in multi-component non-ideal open systems is presented in a classical way, i.e., presenting data, physical laws, initial and boundary conditions and finally the unknowns to be calculated.

*Data*

1. *M*_{1}> , ,0*… M*_{r}*> - molar masses of the elements, where r - is the number of *0
components in the system;

2. Λ > - a position of the right end of the system (its right border – see Figure 1); 0

3. ^{0}_{1} = ^{0}_{1}( )*x …*, ,^{0}* _{r}* =

^{0}

*( )*

_{r}*x*- the initial distributions of the components

[ ] 1

*i*: −Λ, Λ → _{+}, = , ,*i* *… r*

0 , such that:

1

1

*r*

*i*

*i* *i*

*c* *const*

= *M*

=

### ∑

^{0}= .

where 0*c*> is the molar concentration of the system;

4. *D*1^{∗} =*D*1^{∗}

### ( )

, ,*… D*

*r*

^{∗}=

*D*

*r*

^{∗}

### ( )

- self diffusion coefficients of the components, which may depend on components’ densities, = ,### (

1*…*

*r*

### )

;5. *a*1=*a*1

### ( )

, , =*… a*

*r*

*a*

*r*

### ( )

- the activities of the components as functions of components’ densities;6. *ˆt* - the time of the process duration;

7. *j** _{iL}*,

*j*

*[0 ], →*

_{iR}*t*ˆ

*i*= , ,1

*… r*- evolution of mass flow of the

*i*-th component through the left and right boundary. As a consequence of constant concentration of the system these fluxes satisfy the following relation:

1 1

1 ( ) 1 ( ) [0 ]ˆ

*r* *r*

*iL* *iR*

*i* *i* *i* *i*

*j* *t* *j* *t* *for t* *t*

*M* *M*

= =

= ∈ , .

### ∑ ∑

Therefore only 2*r*−1 fluxes are independent.

*Physical Laws*

1. Law of the mass conservation of an *i*-th element. That law tells that a local change of
density of an *i*-th element is a result of its net in- or outflow only:

0 1

*i* *J**i*

*i* *… r*

*t* *x*

∂ ∂

+ = = , , .

∂ ∂ ^{ (1) }

Following Darken’s drift flow idea [1], it is postulated that the flux of an *i*-th element,

*J , is a sum of its diffusion flux, **i* *J*_{i}* ^{d}*, and the drift flux,

### ( )

*i*υ :

*i*

*d*

*i* *i*

*J* :=*J* + υ. (2)

In the next sections it will be shown that the effective solution of Darken’s model for multi-component systems can be obtained when the diffusion flux is expressed by [22]:

*d*

*i* *i i* *j*

*j*

*J* =*B*

### ∑

*F*,

^{ (3) }

where *B is the mobility of an *_{i}*i*-th element and

### ∑

_{j}*F*

*- the sum of the internal or external forces which act on a system.*

_{j}2. A postulate of the constant molar volume of the system. Consequently the molar concentration of the system being a sum of the concentrations of all elements at any position for every time is constant:

1 1

1 1

*r*
*r*

*c* *const*

*M* + ... +*M* = = . (4)

*Initial and boundary conditions*

1. The initial density distributions of the components in the system:

( )^{0}_{i}*x* = * _{i}*(0 ),

*x*

*for x*∈ −Λ, Λ , = , , .[ ]

*i*1

*… r*

2. The following boundary conditions are postulated:

### ( )

^{( )}

### ( )

^{( )}

[0 ]ˆ 1

*i* *iL* *i* *iR*

*J t* *j* *t* *J t* *j* *t*

*for t* *t* *i* *… r*

, −Λ = , , +Λ = ,

∈ , , = , , . (5)

In the open system the functions, ( )*j*_{iL}*t and * *j** _{iR}*( )

*t , have to be known. They can be*calculated e.g., from the known rate of reactions at the boundary or from the experimental data. In the closed system the gradients of all the components at both boundaries vanish, i.e., the flux of an

*i*-th component at the boundary equals zero:

### ( )

^{0}

^{[0 ]}

^{ˆ}

^{1}

*J t**i* , ±Λ = *for t*∈ , , = , , . *t* *i* *… r*

*The unknowns*

1. Densities of the components as functions of time and position, (_{i}*t x*, , = , , . ) *i* 1*… r*
2. A drift velocity as a function of time and position, υ(*t x*, ).

### The Diffusion Flux Formula

In this section the Eq. (3) describing the diffusion flux will be rearranged into the form, which allows obtaining an effective numerical solution. It is generally accepted, that the diffusion force in the Eq. (3) can be described as the spatial gradient of the chemical potential,

µ*i*, and the corresponding flux can be expressed by the following expression

*d* *i*

*i* *i i*

*J* *B*

*x*
µ

= − ∂ .

∂ ^{ (6) }

The thermodynamic definition of the chemical potential is

### (

1### )

*ln*

^{o}### (

1### )

*i* *…* *r* *i* *kT* *a**i* *…* *r*

µ , , =µ + , , , (7)

*where k – the Boltzmann’s constant, T* – an absolute temperature and µ_{i}* ^{o}* is the standard-
state chemical potential usually referred to unit thermodynamic activity (

*a*

*= . The gradient 1) of the chemical potential can be calculated as follows*

_{i}### ( )

1

( )

*r*

*i* *i* *j*

*j* *j*

*x* *x*

µ µ

=

∂ ∂ ∂

= .

∂

### ∑

∂ ∂^{ (8) }

Using Eqs. (6),(7) and (8) the diffusion flux can be expressed in the form

1

ln

*r*

*j*

*d* *i*

*i* *i* *i*

*j* *j*

*J* *B kT* *a*

= *x*

∂ ∂

= − .

∂ ∂

### ∑

^{ (9) }

Substituting the Nernst-Einstein relation

### (

^{D}

^{i}^{∗}

^{=}

^{B kT}

^{i}### )

into Eq. (9), we get1

ln

*r*

*d* *i* *j*

*i* *i* *i*

*j* *j*

*J* *D* *a*

*x*

∗

=

∂ ∂

= − .

∂ ∂

### ∑

^{ (10) }

Above diffusion flux formula can be rearranged to the final form

1
*r*
*d* *j*

*i* *ij*

*j*

*J* *D*

= *x*

= − ∂ ,

### ∑

∂^{ (11) }

where the partial intrinsic diffusivities, *D** _{ij}*, are defined as follows
( ) ( ) ln

*( )*

^{i}*ij* *i* *i*

*j*

*D* :=*D*^{∗} ρ ^{∂} *a* .

∂ (12)

One can notice that in the ideal system, when activity coefficients equal one, the diffusion flux becomes

*d* *i*

*i* *i*

*J* *D*

*x*

∗ ∂

= − .

∂ ^{ (13) }

### The Solution to the Model

Some mathematical aspects critical for understanding the solution of the model are presented bellow. Obtaining this solution involves several steps:

(1) mathematical reformulation of the problem, (2) formulation of the generalized solution,

(3) numerical solution using Galerkin-like method, which reduce an infinite dimension problem to finite one,

(4) solving the resulting system of ordinary differential equations.

Basic concepts on the generalized solution of interdiffusion model in a simple binary system have been already published [23]. In this section the solution of interdiffusion in

multi-component non-ideal open system is presented.

*Mathematical Reformulation of the Problem *

Let us multiply and add equations (1) of local mass conservation

1

1 1

0.

*r*

*i* *i*

*i* *i* *i*

*J*

*M* *t* *M* *x*

ρ

=

∂ + ∂ =

∂ ∂

### ∑

Taking into account Eq. (4) we get

1

1 0.

*r*
*i*

*i* *i*

*c* *J*

*t* *x* = *M*

∂ ∂

+ =

∂ ∂

### ∑

*Because c const*= (see Eq.(4)) one can notice that

1

1

*r*
*i*

*i* *i*

*M* *J*

### ∑

= does not depend on a position in the system, consequently1

( ) 1 ( , ) ( ) 0, [ , ].

*r*

*i*

*i* *i*

*exists K t* *such that* *J t x* *K t* *for t* *x*

= *cM*

∈

### ∑

= ≥ ∈ −Λ + ΛAfter inserting the expression for the flux ( , )*J t x we have *_{i}

1 1

1 ( ) ( ),

*r* *r*

*k*

*ik* *i*

*i* *i* *k*

*D* *cK t*

*M* *x* υ

= =

∂

⎛− + ⎞=

⎜ ∂ ⎟

⎝ ⎠

### ∑ ∑

and finally after rearrangements

1 1

( ) ^{r}* ^{r}* 1

*( )*

_{ik}*.*

^{k}*k* *i* *i*

*K t* *D*

*cM* *x*

υ

= =

= + ∂

### ∑∑

∂^{ (14) }

For further transformations let us introduce the following notations

( ) 1 ( , ) ,

2

( , ) 1 ( , ) ( ),

*i* *i*

*i*

*i* *i* *i*

*i*

*t* *t x dx*

*cM*

*w t x* *t x* *t*

*cM*

Λ

−Λ

= Λ

= −

### ∫

M

M

(15)

where

### (

, ,### )

0

1 1

( ) ( ) ( ) ,

2 2

*t*
*i*

*i* *i L* *i R*

*i* *i*

*t* *x dx* *j* *j* *d*

*cM* ^{Λ} *cM* τ τ

−Λ

= + −

Λ

### ∫

^{0}Λ

### ∫

M (16)

which means that M* _{i}*( )

*t*is known function of time.

One can notice that the following relations are fulfilled

1 1

( ) 1, ( , ) 0, ( , ) 0 1,..., .

*r* *r*

*i* *i* *i*

*i* *i*

*t* *w t x* *w t x dx* *i* *r*

Λ

= = −Λ

= = = =

### ∑

^{M}

### ∑ ∫

^{ (17) }

Using defined variables (15) we obtain the following expressions

### ( ) ( )

1

1

ˆ ( ) ,

( ) ( ) ,

*r*

*k*

*i* *i* *ik* *i* *i*

*k*
*r*

*k*
*k*

*k*

*w* *D* *w* *w* *w*

*t* *x* *x*

*K t* *d w* *w*
*x*

υ υ

=

=

∂

∂ ∂

+ = − + +

∂ ∂ ∂

= + ∂

∂

### ∑

### ∑

M M

(18)

where

1

ˆ ˆ

*r*

*k*

*k* *ik* *ik* *ik*

*i* *i*

*d* *D* *and D* *M* *D*

= *M*

=

### ∑

=^{. }

According to the standards in modern theory of partial differential equations let us define the
solution to the problem (18) in generalized (weak) sense using an integral formula in the
*special function space V [ 24 ]. From the mathematical point of view we can look at *

( )

*i* *i*

*w* =*w t x, (which is function of two variables) as a function of the time only, t *

### (

1### )

( )( ) ( ) * _{r}*( ) [ ]

*w t x* := *w t x … w t x*, , , , *x*∈ −Λ, Λ ,
so

( ) [0 ]ˆ

*w t* ∈*V* *w*: , → . *t* *V*
*This function takes values in the function space V . *

*Generalized Solution *

After some mathematical calculations the problem of interdiffusion in multi-component non- ideal open systems can be formulated as follows:

*We look for a function: w: , → which satisfies the condition: *[0 ]*t*ˆ *V*

0

0 0 0

( )

( ( ) ) | ( ) ( ) ( ) ,

*t* *t* *t*

*w t* *dx* *w* *dx*

*d* *w* *w* *dxd* *K* *w* *dxd*

*x* *x* *x*

φ φ

φ φ

τ φ τ τ τ τ τ τ τ

Λ Λ

−Λ −Λ

Λ Λ

Λ

−Λ

−Λ −Λ

− =

∂ ∂ ∂

⎛ ⎞

= Γ − ⎜⎝ + ∂ ⎟⎠ ∂ + ∂

### ∫ ∫

### ∫ ∫ ∫

^{A}

^{M( ),}

### ∫ ∫

(19)

*for all t*∈[0, ]*t*ˆ *and* φ*∈ , where V* *u v*=

### ∑

^{r}

_{i}_{=}

_{1}

*u v*

_{i i}*is the standard scalar product in*

^{r}*and*

0 (0)

*w* =*w* *. *

In the above equation A *and* Γ are known functions defined as follows

1

( ) ( ) ^{r}* _{j}*( )

_{j}*j*

*A* *a* *for*

κ ξ κ ξ κ κ ξ κ ξ

=

, = +

### ∑

| , , ∈**,**

^{r}A

where *A*( )κ is a matrix whose exact form depends on the partial intrinsic diffusivities

1

( ) * ^{r}* ( ) ( ) [ ( )],

*j* *ij* *ij*

*i*

*a* κ *D* κ *A*κ *D* κ

=

=

### ∑

, =and Γ = Γ( ,...,_{1} Γ where * _{r}*)

( , ) ( ) ( ) 1 ( , ) 1, , .

*i* *i*

*i*

*t* *K t* *t* *j t* *for i* *r*

Γ ±Λ = M_{i} −*cM* ±Λ = …

*Numerical Solution Using Galerkin Method *

The solution to the problem (19) can be approximated numerically using the standard Faedo- Galerkin method. In this approach equation (19) is projected onto some finite subspace

*V**N* ⊂ . The approximated solution shall satisfy the equation: *V*

0

0 0 0

[0 ]ˆ

( )

( ( ) ) | ( ) ( ) ( )

*N*

*N* *N*

*t* *t* *N* *t*

*N* *N*

*t* *t* *V*

*w t* *dx* *w* *dx*

*d* *w* *w* *dxd* *K* *w* *dxd*

*x* *x* *x*

φ

φ φ

φ φ

τ φ τ τ τ τ τ τ τ

Λ Λ

−Λ −Λ

Λ Λ

Λ−Λ

−Λ −Λ

∀ ∈ , ,∀ ∈

− =

⎛ ∂ ⎞ ∂ ∂

⎜ ⎟

= Γ − + + .

⎜ ∂ ⎟ ∂ ∂

⎝ ⎠

### ∫ ∫

### ∫ ∫ ∫

^{A}

^{M( ),}

### ∫ ∫

(20)

It can be proved that such approximation ( )*w*^{N}_{N}^{∞}_{=}_{1} converges to the exact solution if we take
suitable spaces *V . Without going into mathematical details, we will present briefly the ** _{N}*
method to obtain the approximation of the exact solution in the form of finite sum

( ) * ^{N}*1 ( )

*N*

*i* *i*

*w t* =

### ∑

*i*

_{=}λ

*t*φ , where { }φ

*are the base functions. The details of this method exceed the scope of this paper and can be found [25].*

_{i}There are many possible choices for the base { }φ* _{i}* . In our numerical calculations we
have been using the standard polynomial functions in one variable which proved to be very
efficient:

( )φ_{i}*x* =ϕ* _{l}*( )

*x e*

_{si}where ϕ* _{l}* has the graph of the form - shown in Figure 2 and

*e is some ortogonal base [25].*

*After inserting*

_{s}1 ( ) ( )

*N* *N*

*i* *i*

*w*=

### ∑

*i*

_{=}λ

*t*φ

*t*, with the above defined functions ϕ

*, into the equation(20), after some calculations we finally arrive at the system of nonlinear ordinary differential equations (ODE) for the unknown functions λ( ) ( ( )*

_{i}*t*= λ

_{1}

*t …*, ,λ

*( ))*

_{N}*t*of the form

### ( )

1

0 ,1 1

( ) 3*N* ( , ( )) ( ) * _{ns}*( )

_{n N}*,*

_{s r}*t* *B R t* *t* *with* *t* *t*

λ = ^{−} λ λ = λ _{≤ ≤} _{≤ ≤ −}

Λ

where *B* is a tridiagonal matrix of the form

2 1 0 0

1 4 1

0 1 0

4 1

0 0 1 2

*B*

⎡ ⎤

⎢ ⎥

⎢ ⎥

⎢ ⎥

=⎢ ⎥

⎢ ⎥

⎢ ⎥

⎣ ⎦

…

…

and *R t*^{( , )}λ =

### [

*R t*

*ls*

^{( , )}λ

### ]

_{0}

_{≤ ≤}

*l N*

_{,0}

_{≤ ≤ −}

*s r*

_{1}. The explicit form of the entry

*R t*

*( , )λ is given as follows*

_{ls}0 1 2 3 4

( , ) ( ) ( ) ,

*ls* *s*

*R t* λ =*z* − +*z* *K t z* + + M*z* *t* *e z* (21)

where

### ( )

### ( ) ( )

### ( )

### ( )

## (

0 0 0

1

1 0 1 1

1

2 0 1 0 1

1

3 0 1 1 1 1

1

( ) ( ) ( ) ,

2

( 1)( ) ( )( ) ,

2

1 ( ) ,

2 4 ( 1)

*l* *R* *Nl* *L* *l* *Nl* *s*

*r*

*l* *p* *s* *lp* *l* *p* *Nl* *p* *s* *lp* *l* *p*

*p*

*l* *l* *s* *Nl* *l* *ls* *Nl* *l* *s*

*r*

*l* *p* *l* *p* *l* *s* *lp* *l* *s* *l* *p* *ls*

*p*

*z* *t* *t* *t* *e*

*N*

*z* *N* *D l* *e* *e* *D l e* *e*

*z*

*z* *N* *d l* *e*

δ δ δ δ

δ λ λ δ λ λ

δ λ δ δ λ δ λ

δ λ λ λ λ λ λ

−

− +

=

− +

−

− − − −

=

= Γ − Γ − Λ +

= − − + −

Λ

= + + −

= − − + − +

Λ

### ∑

### ∑

M

### ( ) ( ) )

### ( ) ( )

0 1 1 1 1

1

4 0 1 1

1

( 1) ( ) ( ) ,

( 1) ( ) .

2

*l* *p* *Nl* *p* *lp* *ls* *Nl* *p* *l* *p* *ls* *lp* *l* *s* *l* *p* *l* *s*

*r*

*l* *p* *lp* *l* *p* *Nl* *p* *lp* *l* *p*

*p*

*d l* *e* *d l* *e* *d l* *e*

*z* *N* *d l* *e* *d l* *e*

δ δ λ λ δ λ λ λ λ λ λ

δ λ λ δ λ λ

+ + + +

−

− +

=

+ − + + − + −

= − − + −

Λ

### ∑

(22)

where δ* _{ij}* and δ

*have the following meaning*

_{ij}1 0

, 1

0 1

*ij* *ij* *ij*

*if i* *j* *if i* *j*

*if i* *j* *if i* *j*

δ =^{⎧}⎨⎩ ^{=}≠ δ = −δ =^{⎧}⎨⎩ ≠^{=}

Together with the initial condition λ* ^{o}* (which can be found from

^{0}), this is a standard Cauchy initial problem for ODE:

3 1

( ) ( , ( ))

(0) ^{o}*t* *N* *B R t* *t*

λ λ

λ λ

⎧ = −

⎪ Λ

⎨⎪ =

⎩

(23)

After having solved the above system of ODEs we can compute the approximation of the

profiles *w*^{N}

1

0 1

( , ) ( ) ( ) .

*N* *r*

*N*

*np* *n* *p*

*n* *p*

*w t x* ^{−} λ *t* ϕ *x e*

= =

=

### ∑∑

^{ (24) }

and subsequently using eqs. (15) and (16) compute density profiles of the components ( , )

*i* = *i* *t x* .

### Solving the resulting system of ordinary differential equations

Any numerical method can be applied to solve the system (23) and obtain the values of λ( )*t* .
For this particular system the standard Runge-Kutta of fourth-order with adaptive step size
was chosen. The reason was that the Runge-Kutta method requires relatively small number of

right-hand side evaluations, what was especially important in the above system because right- hand side of the ODE is complex and its evaluation is time consuming. The Runge-Kutta Fehelberg [26] method using special pair Runge-Kutta forth and fifth order method was implemented in our procedure. It needs only 5 evaluation in one step and allows to control the level of accuracy of the solution.

### Modelling interdiffusion in Cu-Fe-Ni Alloy

Formulated above model will be applied for demonstrating the possibility of interdiffusion modelling in non-ideal system. Two different boundary conditions will be analysed:

• interdiffusion in the closed system and

• interdiffusion due to selective oxidation – open system.

For demonstration Cu-Fe-Ni system has been chosen. Cu-Fe-Ni system at 1273 K have a miscibility gap and a wide single phase region (Figure 3). Thermodynamic data for this system has been assessed by Jansson [27] and re-evaluated by Rönka et al [8]. In the Figure 4 some isoactivity curves of copper, iron and nickel at 1273 K are presented. Isoactivity data illustrated in Figure 4 were applied to calculate partial intrinsic diffusivities – Eq. (12) and intrinsic fluxes – Eq. (11).

*Modelling Interdiffusion in the Cu-Fe-Ni Closed System *

Interdiffusion modelling in the Cu-Fe-Ni closed system has been done using DifSim software [28] and compared with the experimental results [21]. For the calculations the following data have been used:

(1) Initial concentration profiles – step functions defined by the terminal composition of the diffusion couple, see Figure 5.

42 .% [ ,0]

0 .% ]0, ]

*wt* *x*

*Cu* *wt* *x*

⎧ ∈ −Λ

= ⎨⎩ ∈ Λ , 0 .% [ ,0]

24 .% ]0, ]

*wt* *x*

*Fe* *wt* *x*

⎧ ∈ −Λ

= ⎨⎩ ∈ Λ , 58 .% [ ,0]

76 .% ]0, ]

*wt* *x*

*Ni* *wt* *x*

⎧ ∈ −Λ

= ⎨⎩ ∈ Λ

(2) Average molar concentration of the Cu-Fe-Ni alloy, *c*=0.144*mol cm*^{−}^{3}.
(3) Thickness of the diffusion couple, 2Λ =*0.07 cm*.

(4) Calculated average self-diffusion coefficients of copper, iron and nickel in Cu-Fe-Ni diffusion couple [21] at 1273 K

11 2 1

11 2 1

11 2 1

2.89 10 1.52 10 2.09 10

*Cu*

*Fe*

*Ni*

*D* *cm s*

*D* *cm s*

*D* *cm s*

− −

− −

− −

= ⋅

= ⋅

= ⋅

(5) Thermodynamic activity data – Figure 4.

(6) Time of the process duration, ˆ 612*t* = *ks*.

In the Figure 5 the calculated concentration profiles of Cu, Fe and Ni are compared with the experimental results and show satisfactory agreement.

The next figure shows calculated concentration profiles of Cu, Fe and Ni in 48Ni- 52Cu/19.7Ni-80.3Fe (wt. %) diffusion couple for a chemical potential gradient as a driving force for diffusion – Eq . (9) and assuming that system is ideal – Eq. (13). One can notice that calculated concentration profiles depend on the used flux formula. Consequently, the

assumption of “ideality” of the system – i.e., neglecting of thermodynamic data – can strongly affect the calculated concentration profiles.

In the Figure 7 some calculated and experimental diffusion paths for Cu-Fe-Ni system at 1273 K are assembled.

*Selective oxidation of Cu-Fe-Ni Alloy – Open System *

Initially uniform alloy changes its composition near the alloy/scale boundary due to the oxidation process. In multi-component alloy the chemical reaction (oxide formation) at the boundary effects concentration of all the elements in the alloy. Modelling of such process involves formulation of the proper boundary conditions.

*The flux of component at the boundary, (i.e. for x*= Λ ),which is oxidised (forms a
scale) can be expressed as follows

( , ) * ^{diff}*( , ) ( , ) ( ),

*i* *i* *i*

*J t* *J* *t* *c t* *d X* *t*

*dt*

Λ = Λ + Λ ∆ (25)

where /*d X dt*∆ is the rate of the alloy consumption due to oxidation.

If some element in the alloy does not form a scale then its flux through the boundary equals zero

( , ) 0*J t** _{i}* Λ = (26)

and consequently

( , ) ( , ) ( ).

*diff*

*i* *i*

*J* *t* *c t* *d X* *t*

*dt*

Λ = − Λ ∆ (27)

If the scale (oxide) is compact and adheres to the alloy, the rate of the alloy consumption is inversely proportional to instantaneous thickness of the oxide layer, which in turn is

proportional to the displacement of the alloy surface ∆*X*. Thus the rate of the alloy
consumption is

*k**c*

*d X*

*dt* *X*

∆ =

∆ ^{ (28) }

where *k is a parabolic rate constant of an alloy consumption. The displacement of the alloy ** _{c}*
surface due to oxidation can be obtained solving the equation (28)

2 _{C}

*X* *k t*

∆ = (29)

and consequently

2 .
*k**c*

*d X*

*dt* *t*

∆ = (30)

Expressions (25), (26) and (30) introduced into equations (5) describe boundary conditions for the selective oxidation.

In this section modelling of interdiffusion in a selectively oxidised Cu-50Fe-40Ni (wt.%) alloy at 1273 K is demonstrated. For the calculations the following data have been used:

(1) Initial concentration profiles – uniform concentration profiles:

(0, ) 10 .%

(0, ) 50 .%

(0, ) 40 .%

[ , ]

*Cu*

*Fe*
*Ni*

*c* *x* *wt*

*c* *x* *wt*

*c* *x* *wt*

*for x*

=

=

=

∈ −Λ Λ

(2) Average molar concentration of the Cu-Fe-Ni alloy, *c*=0.144*mol cm*^{−}^{3}.
(3) Thickness of the diffusion couple, 2Λ =*0.06 m*µ .

(4) Average self-diffusion coefficients of copper, iron and nickel in Cu-Fe-Ni at 1273 K (see above)

(5) Thermodynamic activity data – Figure 4.

(6) Parabolic rate constant of an alloy consumption [29], *k** _{c}* =3.5 10⋅

^{−}

^{7}

*cm s*

^{2}

^{−}

^{1}.

In the Figure 8 the calculated concentration profiles of copper, iron and nickel due to iron selective oxidation of Cu-Fe-Ni are presented. After initial enrichment of the alloy in nickel its concentration decreases for longer times.

In the figure 9 the diffusion paths of the selectively oxidised Cu-Fe-Ni alloy are shown.

This figure illustrates the fact that due to oxidation process initially single-phase alloy can change to multi-phase when the diffusion path crosses miscibility gap and cross over to a two phase region.

### Summary and Conclusions

1. Mathematical model of interdiffusion in multi-component, non-ideal open systems has been formulated. For the known thermodynamic data (components’ activities), kinetic data (self diffusivities) and reaction rate at the boundary (fluxes of the components) the evolution of the concentration profiles and drift velocity can be found.

2. Using idea of generalized solution and Galerkin approximation, the numerical solution to the model has been obtained. Complicated system of non-linear partial differential

equations (PDE) describing interdiffusion process has been transformed to the system of ordinary differential equations (ODE), which is much simpler to solve.

3. Effective formulae enable to calculate the concentration profiles of the elements and the drift velocity as a function of time and position have been presented.

4. The model can be used both for a quantitative description of interdiffusion in the open and closed systems.

5. Application of the model for modelling interdiffusion in the Cu-Fe-Ni diffusion couple (closed system) was demonstrated. The calculated concentration profiles were consistent with experimental results

6. Iron selective oxidation of Cu-50Fe-40Ni alloy was chosen to demonstrate modelling interdiffusion in the open system. It was demonstrated that initially single-phase alloy can change to multi-phase due to oxidation process when the diffusion path crosses miscibility gap and cross over to a two phase region.

7. These examples show the potential of the model in describing interdiffusion in a wide range of diffusion limited process. An effective application of the model involves knowledge of the thermodynamic and kinetic data. Kinetic data – self diffusivities – can be obtained using e.g. radiotracer technique [30] or using inverse methods [31].

Significant progress is observed in the software. Programs like Thermo-Calc [32],

FactSage [33] etc. can be used as an effective tool for obtaining thermodynamic activities even in a multi-component systems.

8. So far results and analysis of general flux formulae – Eq. (3) – show prospect of the extension of this model in modelling stresses affected diffusion, electromigration, diffusion in electrolytes, etc.

### Acknowledgments

This work was supported by the Polish State Committee for Scientific Research Grants No.

4T08A 001 25 during the period (2003-2005) and No. 10.10.160. 975. The author is indebt to Professor M. Danielewski (AGH University of Science and Technology) for stimulating discussions and K. Szyszkiewicz (WSB-NLU Nowy Sącz) for mathematical assistance.

### References

[1] L.S. Darken, Trans. AIME, 180, 430 (1948) [2] L. Onsager, Phys. Rev., 38, 2265 (1931)

[3] J.S. Kirkaldy: series of articles in Can. J. Phys (1957-1969)

[4] J.S. Kirkaldy and D.J. Young, Diffusion in The Condensed State, The Institure of Metals, London (1987)

[5] M.A. Dayananda, in Diffusion in Solid Metals and Alloys, Landolt-Börnstein, Numerical Data and Functional Relationships in Science and Technology, New Series III/26, Ed., H.

Mehrer, Springer-Verlag, Berlin (1991)

[6] M.A. Dayananda, in Proc. Symp. Diffusion in Solids. Recent Developments, Metall. Soc.

of AIME 195-, Warrendale, PA, 1984, Eds., M.A. Dayannada and G.E. Murch (eds), Detroit, USA (1985)

[7] F.J.J. van Loo, Proc. Solid St. Chem., 20, 1251 (1990)

[8] K.J. Ronka, A.A. Kodentsov, P.J.J. Van Loon, J.K.Kivilahti, F.J.J. Van Loo, Metall. and Materials Transactions A, 27A, 2229 (1996)

[9] M.S. Thomson and J.E. Morral, Acta metall., Vol. 34, No. 2, 339 (1986) [10] J.E. Morral and H. Chen, Scripta mater., 43, 699 (2000)

[11] C.E. Campbel, W.J. Boettinger and U.R.Kattner, Acta Materialia, 50, 775 (2002) [12] T. Helander and J. Agren, Acta mater., Vol. 47, No. 11, 3291 (1999)

[13] M.A. Dayananda, Deffect and Diffusion Forum, 83, 73 (1992) [14] M.A. Dayannda, Mater. Sci. Eng., A121, 351 (1989)

[15] C. Cserhati, U. Ugaste, M.J.H. van Dal, N.J.H.G.M. Lousberg, A.A. Kodentsov and F.J.J.

van Loo, Deffect and Diffusion Forum, 194-199, 189 (2001)

[16] S.R. de Groot and P. Mazur, Non-Equilibrium Thermodynamics, Dover Publications, Inc., New York (1984)

[17] A.C. Smigelskas and E.O. Kirkendall, Trans. AIME, 171, 2071 (1947) [18] K. Holly and M. Danielewski, Phys. Review B, 50, 13336 (1994)

[19] M. Danielewski, K. Holly and W. Krzyzanski, Polish J. Chem. 68, 2031 (1994) [20] M. Danielewski, R. Filipek, K. Holly and B. Bozek, phys. stat. sol (a) 145, 339 (1994) [21] R. Bachorczyk, M. Danielewski, R. Filipek, Defect and Diffusion Forum, 216-217, 141 (2003)

[22] M. Planck, Ann. Phys. Chem. (Wiedemann) 39, 161 (1890)

[23] M. Danielewski and R. Filipek, J. Comp. Chem., Vol. 17, No. 13, 1497 (1996)

[24] J. L. Lions, E. Magenes, "Non-homogeneous boundary value problems and applications", Springer-Verlag, Berlin (1972)

[25] R. Filipek and K. Szyszkiewicz, “Numerical solution to the Interdiffusion Problem in Multi-component Non-ideal Open Systems”, in Proc. of International Conference DIMAT 2004, Trans. Tech, Defect and Diffusion Forum, to be published (2005)

[26] E. Fehlberg, Computing 4, 93 (1969)

[27] A. Jansson: TRITA-MAC-0340, The Royal Institute of Technology Stockholm, 1-14 (1987)

[28] Demonstration version of the software is available at the web site http://ceramrtr.ceramika.agh.edu.pl/~rof/demo.html

[29] Z. Grzesik, PhD Thesis, Krakow (1992)

[30] St. Frank, U. Södervall and Chr. Herzig, Phys. Stat. Sol (b), 191 45 (1995)

[31] S. Datta, R. Filipek and M. Danielewski, Defect and Diffusion Forum, 203-205, 47 (2002)

*[32] Thermo-Calc is a registered trade mark of Thermo-Calc Software. *

*[33] FactSage is a registered trade mark of ESM Software, Inc. *

### Figure Captions

**Figure 1** Schematic graph of interdiffusion in a binary diffusion couple A/B: (a) initial state –

*initial density profile of the component A, ( )*^{0}_{A}*x* at *t*= , (b) density profile ( )0 _{A}*x after some *
time 0*t*> and (c) for long time *t* 0.

**Figure 2** Graphical representation of the base functions ϕ* _{k}*( )

*x*. The interval [−Λ Λ, ] was

*divided into N equal subintervals*[ ,

*x x*

_{k}

_{k}_{+}

_{1}] where

*k*=0, ,…

*N*−1. Nodes

*x*

*= −Λ +*

_{k}*k*(2 / )Λ

*N*define triangular-like functions ϕ

*( )*

_{k}*x*.

**Figure 3** Ternary phase diagram Cu-Fe-Ni at 1273 K: 1 – single phase alloy, 2 – two phase
alloy. The miscibility gap based on experimental results and thermodynamic reassessment [8]

**Figure 4** Calculated isoactivity curves for Cu, Fe and Ni at 1273 K based on pure element
reference state at 1273 K (1 atm) [8].

**Figure 5** The calculated (solid lines) and experimental concentration profiles of the
components in Cu-Fe-Ni alloy after 612 ks of diffusion annealing at 1273 K in argon.

**Figure 6** The comparison of calculated concentration profiles using different flux formulae:

(a) for a chemical potential gradient as a driving force for diffusion (points) and (b) assuming the system is ideal (dashed lines).

**Figure 7** The comparison of the calculated and experimental diffusion paths in the Cu-Fe-Ni
systems at 1273 K.

**Figure 8** The calculated Cu, Fe and Ni concentration profiles in selectively (iron) oxidised
Cu-50Fe-40Ni alloy at 1273 K.

**Figure 9** The diffusion paths in profiles in selectively (iron) oxidised Cu-50Fe-40Ni alloy at
1273 K

### Figures

**Figure 1** Schematic graph of interdiffusion in a binary diffusion couple A/B: (a) initial state
*– initial density profile of the component A, ( )*^{0}_{A}*x* at *t*= , (b) density profile ( )0 _{A}*x after *
some time *t* > and (c) for long time 0 *t* 0.

### ϕ

_{0}

### ϕ

_{k}### ϕ

_{N}*x*

_{0}

*x*

_{1}

*x*

_{k}_{−1}

*x*

_{k}*x*

_{k}_{+1}

*x*

_{N}_{−1}

*x*

_{N}**Figure 2** Graphical representation of the base functions ϕ* _{k}*( )

*x*. The interval [−Λ Λ, ] was

*divided into N equal subintervals*[ ,

*x x*

_{k}

_{k}_{+}

_{1}] where

*k*=0, ,…

*N*−1. Nodes

*x*

*= −Λ +*

_{k}*k*(2 / )Λ

*N*define triangular-like functions ϕ

*( )*

_{k}*x*.

**2**
**1**

**Fe wt. %**

**Ni**

**Fe**
**Cu**

**Figure 3** Ternary phase diagram Cu-Fe-Ni at 1273 K: 1 – single phase alloy, 2 – two phase
alloy. The miscibility gap based on experimental results and thermodynamic

reassessment [8]

**0.95**

**0.6**

**0.85**
**0.925****0.9**

**0.8**
**0.7**

**0.5**
**0.1**

**0.3**
**0.4**

**0.2**

**Fe at. %**

**Ni**

**Cu** **Fe**

**a**

_{Cu}**0.7**

**0.9**
**0.95**
**0.8**
**0.6**
**0.3**

**0.4**
**0.5**
**0.2**
**0.1**
**0.05**

**Fe wt. %**

**Ni**

**Cu** **Fe**

**a**

**Fe**

**Fe wt. %**

**0.1**
**0.25**
**0.4**
**0.5**

**0.05**
**0.15**
**0.2**
**0.3**
**0.6**
**0.7**
**0.8**
**0.9**

**Ni**

**Fe**
**Cu**

**a**

_{Ni}**Figure 4** Calculated isoactivity curves for Cu, Fe and Ni at 1273 K based on pure element
reference state at 1273 K (1 atm) [8].

**-200** **-100** **0** **100** **200**
**0**

**10**
**20**
**30**
**40**
**50**
**60**
**70**
**80**

** Initial profiles**
Eksperiment

** Fe**
** Ni**
** Cu**

** Calculations**

Cu, Fe, Ni, wt. %

**x, **µ**m**

**Figure 5** The calculated (solid lines) and experimental concentration profiles of the
components in Cu-Fe-Ni alloy after 612 ks of diffusion annealing at 1273 K in argon.

-300 -200 -100 0 100 200 300

0 10 20 30 40 50 60

Fe Ni

Cu, Fe, Ni, wt. %

x, µm

Non-ideal

Ideal

Cu

**Figure 6** The comparison of calculated concentration profiles using different flux formulae:

(a) for a chemical potential gradient as a driving force for diffusion (points) and (b) assuming the system is ideal (dashed lines).

Fe, wt %

Ni

Cu Fe

Experimental Calculated

**Figure 7** The comparison of the calculated and experimental diffusion paths in the Cu-Fe-Ni
system at 1273 K.

**0.010** **0.015** **0.020** **0.025** **0.030**
0

20 40 60 80

distance, µm

Cu, at. %

0 20 40 60

Fe, at. %

20 40 60

0.0001 s 0.0003 s 0.0005 s

Ni, at. %

**Figure 8** The calculated Cu, Fe and Ni concentration profiles in selectively (iron) oxidised
10Cu-50Fe-40Ni alloy at 1273 K.

t5

t4

t3

t1

**Fe wt. %**

Ni

Cu Fe

t2

**Figure 9** The diffusion paths in profiles in selectively (iron) oxidised 10Cu-50Fe-40Ni alloy
at 1273 K, *t*_{1}< < < < . *t*_{2} *t*_{3} *t*_{4} *t*_{5}